|Palladium in the periodic table|
|Name, symbol, number||palladium, Pd, 46|
|Element category||transition metal|
|Group, period, block||10, 5, d|
|Standard atomic weight||106.42|
|Electron configuration||[Kr] 4d10
2, 8, 18, 18
|Density (near r.t.)||12.023 g·cm−3|
|Liquid density at m.p.||10.38 g·cm−3|
|Melting point||1828.05 K, 1554.9 °C, 2830.82 °F|
|Boiling point||3236 K, 2963 °C, 5365 °F|
|Heat of fusion||16.74 kJ·mol−1|
|Heat of vaporization||358 kJ·mol−1|
|Molar heat capacity||25.98 J·mol−1·K−1|
|Oxidation states||0, +1, +2, +4
(mildly basic oxide)
|Electronegativity||2.20 (Pauling scale)|
|Ionization energies||1st: 804.4 kJ·mol−1|
|2nd: 1870 kJ·mol−1|
|3rd: 3177 kJ·mol−1|
|Atomic radius||137 pm|
|Covalent radius||139±6 pm|
|Van der Waals radius||163 pm|
|Crystal structure||face-centered cubic|
|Electrical resistivity||(20 °C) 105.4 nΩ·m|
|Thermal conductivity||71.8 W·m−1·K−1|
|Thermal expansion||(25 °C) 11.8 µm·m−1·K−1|
|Speed of sound (thin rod)||(20 °C) 3070 m·s−1|
|Young's modulus||121 GPa|
|Shear modulus||44 GPa|
|Bulk modulus||180 GPa|
|Vickers hardness||461 MPa|
|Brinell hardness||310 MPa|
|CAS registry number||7440-05-3|
|Naming||after asteroid Pallas, itself named after Pallas Athena|
|Discovery||William Hyde Wollaston (1803)|
|First isolation||William Hyde Wollaston (1803)|
|Most stable isotopes|
|Main article: Isotopes of palladium|
Palladium is a chemical element with the chemical symbol Pd and an atomic number of 46. It is a rare and lustrous silvery-white metal discovered in 1803 by William Hyde Wollaston. He named it after the asteroid Pallas, which was itself named after the epithet of the Greek goddess Athena, acquired by her when she slew Pallas. Palladium, platinum, rhodium, ruthenium, iridium and osmium form a group of elements referred to as the platinum group metals (PGMs). These have similar chemical properties, but palladium has the lowest melting point and is the least dense of them.
Over half of the supply of palladium and its congener platinum goes into catalytic converters, which convert up to 90% of harmful gases from auto exhaust (hydrocarbons, carbon monoxide, and nitrogen dioxide) into less-harmful substances (nitrogen, carbon dioxide and water vapor). Palladium is also used in electronics, dentistry, medicine, hydrogen purification, chemical applications, groundwater treatment and jewelry. Palladium plays a key role in the technology used for fuel cells, which combine hydrogen and oxygen to produce electricity, heat, and water.
Ore deposits of palladium and other PGMs are rare, and the most extensive deposits have been found in the norite belt of the Bushveld Igneous Complex covering the Transvaal Basin in South Africa, the Stillwater Complex in Montana, United States, the Thunder Bay District of Ontario, Canada, and the Norilsk Complex in Russia. Recycling is also a source of palladium, mostly from scrapped catalytic converters. The numerous applications and limited supply sources of palladium result in the metal attracting considerable investment interest.
Palladium belongs to group 10 in the periodic table, but has a very atypical configuration in its outermost electron shells compared to the other members of group 10 (see also niobium (41), ruthenium (44), and rhodium (45)), having fewer filled electron shells than the elements directly preceding it (a phenomenon unique to palladium). This makes its valence shell have 10 more electrons than the noble gases.
|Z||Element||No. of electrons/shell|
|28||nickel||2, 8, 16, 2 or 2, 8, 17, 1|
|46||palladium||2, 8, 18, 18|
|78||platinum||2, 8, 18, 32, 17, 1|
|110||darmstadtium||2, 8, 18, 32, 32, 16, 2 (predicted)|
Palladium is a soft silver-white metal that resembles platinum. It is the least dense and has the lowest melting point of the platinum group metals. It is soft and ductile when annealed and greatly increases its strength and hardness when it is cold-worked. Palladium dissolves slowly in concentrated nitric acid, in hot, concentrated sulfuric acid, and, when finely divided, in hydrochloric acid.
Common oxidation states of palladium are 0, +1, +2 and +4. There are relatively few known compounds with palladium unambiguously in the +3 oxidation state, though such compounds have been proposed as intermediates in many palladium-catalyzed cross-coupling reactions. In 2002, palladium(VI) was first reported.
Naturally occurring palladium is composed of seven isotopes, which includes six stable isotopes. The most stable radioisotopes are 107Pd with a half-life of 6.5 million years (found in nature), 103Pd with a half-life of 17 days, and 100Pd with a half-life of 3.63 days. Eighteen other radioisotopes have been characterized with atomic weights ranging from 90.94948(64) u (91Pd) to 122.93426(64) u (123Pd). Most of these have half-lives that are less than thirty minutes, except 101Pd (half-life: 8.47 hours), 109Pd (half-life: 13.7 hours), and 112Pd (half-life: 21 hours).
For isotopes with atomic mass unit values less than that of the most abundant stable isotope, 106Pd, the primary decay mode is electron capture with the primary decay product being rhodium. The primary mode of decay for those isotopes of Pd with atomic mass greater than 106 is beta decay with the primary product of this decay being silver.
Radiogenic 107Ag is a decay product of 107Pd and was first discovered in 1978 in the Santa Clara meteorite of 1976. The discoverers suggest that the coalescence and differentiation of iron-cored small planets may have occurred 10 million years after a nucleosynthetic event. 107Pd versus Ag correlations observed in bodies, which have been melted since accretion of the solar system, must reflect the presence of short-lived nuclides in the early solar system.
Palladium does not react with oxygen at normal temperatures (and thus does not tarnish in air). Palladium heated to 800°C will produce a layer of palladium(II) oxide (PdO). It lightly tarnishes in a moist atmosphere containing sulfur.[clarification needed] Palladium primarily exists in the 0, +2, and +4 oxidation states; the +4 oxidation state is comparatively rare. One major example of palladium(IV) is hexachloropalladate(IV), [PdCl6]2−.
Elemental palladium reacts with chlorine to give palladium(II) chloride; it dissolves in nitric acid and precipitates palladium(II) acetate on addition of acetic acid. These two compounds and the bromide are reactive and relatively inexpensive, making them convenient entry points to palladium chemistry. All three are not monomeric; the chloride and bromide often must be refluxed in acetonitrile to obtain the more reactive acetonitrile complex monomers, for example:
- PdX2 + 2 MeCN → PdX2(MeCN)2 (X = Cl, Br)
Palladium(II) chloride is the principal starting material for many other palladium catalysts. It is used to prepare heterogeneous palladium catalysts: palladium on barium sulfate, palladium on carbon, and palladium chloride on carbon. It reacts with triphenylphosphine in coordinating solvents to give bis(triphenylphosphine)palladium(II) dichloride, a useful catalyst. Where desired, the catalyst may be formed in situ.
- PdCl2 + 2 PPh3 → PdCl2(PPh3)2
- 2 PdCl2(PPh3)2 + 4 PPh3 + 5 N2H4 → 2 Pd(PPh3)4 + N2 + 4 N2H5+Cl−
The great many reactions in which palladium compounds serve as catalysts are collectively known as palladium-catalyzed coupling reactions. Prominent examples include the Heck, Suzuki and Stille reactions. Palladium(II) acetate, tetrakis(triphenylphosphine)palladium(0) (Pd(PPh3)4, and tris(dibenzylideneacetone)dipalladium(0) (Pd2(dba)3) are useful in this regard, either as catalysts or as starting points to catalysts.
William Hyde Wollaston noted the discovery of a new noble metal in July 1802 in his lab-book and named it palladium in August of the same year. Wollaston purified enough of the material and offered it, without naming the discoverer, in a small shop in Soho in April 1803. After harsh criticism that palladium is an alloy of platinum and mercury by Richard Chenevix, Wollaston anonymously offered a reward of 20 British pounds for 20 grains of synthetic palladium alloy. Chenevix received the Copley Medal in 1803 after he published his experiments on palladium. Wollaston published the discovery of rhodium in 1804 and mentions some of his work on palladium. He disclosed that he was the discoverer of palladium in a publication in 1805.
It was named by Wollaston in 1802 after the asteroid Pallas, which had been discovered two months earlier. Wollaston found palladium in crude platinum ore from South America by dissolving the ore in aqua regia, neutralizing the solution with sodium hydroxide, and precipitating platinum as ammonium chloroplatinate with ammonium chloride. He added mercuric cyanide to form the compound palladium(II) cyanide, which was heated to extract palladium metal.
Palladium chloride was at one time prescribed as a tuberculosis treatment at the rate of 0.065 g per day (approximately one milligram per kilogram of body weight). This treatment had many negative side-effects, and was later replaced by more effective drugs.
In the run up to 2000, the Russian supply of palladium to the global market was repeatedly delayed and disrupted because the export quota was not granted on time, for political reasons. The ensuing market panic drove the price to an all-time high of $1100 per troy ounce in January 2001. Around this time, the Ford Motor Company, fearing auto vehicle production disruption due to a possible palladium shortage, stockpiled large amounts of the metal purchased near the price high. When prices fell in early 2001, Ford lost nearly US$1 billion. World demand for palladium increased from 100 tons in 1990 to nearly 300 tons in 2000. The global production of palladium from mines was 222 tonnes in 2006 according to the United States Geological Survey. Most palladium is used for catalytic converters in the automobile industry. There are currently concerns about a steady supply of palladium in the wake of Russia’s military maneuvers in Ukraine, partly as sanctions could hamper Russian palladium exports; any restrictions on Russian palladium exports would exacerbate what is already expected to be a large palladium deficit in 2014. 
In 2007, Russia was the top producer of palladium, with a 44% world share, followed by South Africa with 40%. Canada with 6% and the U.S. with 5% are the only other substantial producers of palladium.
Palladium can be found as a free metal alloyed with gold and other platinum-group metals in placer deposits of the Ural Mountains, Australia, Ethiopia, North and South America. For the production of palladium these deposits play only a minor role. The most important commercial sources are nickel-copper deposits found in the Sudbury Basin, Ontario, and the Norilsk–Talnakh deposits in Siberia. The other large deposit is the Merensky Reef platinum group metals deposit within the Bushveld Igneous Complex South Africa. The Stillwater igneous complex of Montana and the Roby zone ore body of the Lac des Îles igneous complex of Ontario are the two other sources of palladium in Canada and the United States. Palladium is found in the rare minerals cooperite and polarite.
Palladium is also produced in nuclear fission reactors and can be extracted from spent nuclear fuel (see synthesis of precious metals) though this source for palladium is not used. None of the existing nuclear reprocessing facilities are equipped to extract palladium from the high-level radioactive waste.
The largest use of palladium today is in catalytic converters. Palladium is also used in jewelry, in dentistry, watch making, in blood sugar test strips, in aircraft spark plugs and in the production of surgical instruments and electrical contacts. Palladium is also used to make professional transverse flutes. As a commodity, palladium bullion has ISO currency codes of XPD and 964. Palladium is one of only four metals to have such codes, the others being gold, silver and platinum. Palladium was also used in the cold fusion experiments that promised but failed to prove net energy production in and after 1989.
When it is finely divided, such as in palladium on carbon, palladium forms a versatile catalyst and speeds up hydrogenation and dehydrogenation reactions, as well as in petroleum cracking. A large number of carbon-carbon bond forming reactions in organic chemistry (such as the Heck reaction and Suzuki coupling) are facilitated by catalysis with palladium compounds. (see Palladium Compounds and palladium-catalyzed coupling reactions) In addition, palladium, when dispersed on conductive materials, proves to be an excellent electrocatalyst for oxidation of primary alcohols in alkaline media. In 2010, palladium-catalysed organic reactions were recognised by the Nobel Prize in Chemistry. Palladium is also a versatile metal for homogeneous catalysis. It is used in combination with a broad variety of ligands for highly selective chemical transformations. A 2008 study showed that palladium is an effective catalyst for making carbon-fluoride bonds. Palladium is found in the Lindlar catalyst, also called Lindlar's Palladium.
The second-biggest application of palladium in electronics is in the manufacture of multilayer ceramic capacitors, in which palladium (and palladium-silver alloys) are used as electrodes. Palladium (sometimes alloyed with nickel) is used in connector platings in consumer electronics.
It is also used in plating of electronic components and in soldering materials. The electronic sector consumed 1.07 million troy ounces (33.2 tonnes) of palladium in 2006, according to a Johnson Matthey report.
Hydrogen easily diffuses through heated palladium; thus, it provides a means of purifying the gas. Membrane reactors with Pd membranes are therefore used for the production of high purity hydrogen. Palladium is a part of the palladium-hydrogen electrode in electrochemical studies. Palladium(II) chloride can oxidize large amounts of carbon monoxide gas, and is used in carbon monoxide detectors.
Palladium readily absorbs hydrogen at room temperatures forming palladium hydride PdHx with x below 1. While this property is common to many transition metals, palladium is unique by the high absorption capacity and by that it does not lose its ductility until high x values. This property has been investigated for designing an efficient, yet inexpensive hydrogen storage material (palladium itself is prohibitively expensive for this purpose).
Palladium itself has been used as a precious metal in jewelry since 1939, as an alternative to platinum for making white gold. This use resulted from the naturally white color of palladium, which required no rhodium plating. Palladium is proportionally much lighter than platinum. Similar to gold, palladium can be beaten into a thin leaf form as thin as 100 nm (1/250,000 in). Unlike platinum, palladium may discolor upon heating to above 400 °C (752 °F); it is relatively brittle and reacts with strong acids such as nitric acid.
Palladium is one of the three most popular metals used to make white gold alloys (nickel and silver can also be used). Palladium-gold is a more expensive alloy than nickel-gold, but seldom causes allergic reactions (though certain cross-allergies with nickel may occur).
When platinum was declared a strategic government resource during World War II, many jewelry bands were made out of palladium. As recently as September 2001, palladium was more expensive than platinum and rarely used in jewelry also due to the technical obstacle of casting. However, the casting problem has been resolved and its use in jewelry has increased because of a large spike in the price of platinum and a drop in the price of palladium.
Prior to 2004, the principal use of palladium in jewelry was the manufacture of white gold. In early 2004, when gold and platinum prices rose steeply, China began fabricating significant volumes of palladium jewelry and used 37 tonnes of palladium for this purpose in 2005. Changes of the relative price between palladium and platinum after 2008 lowered demand for palladium to 17.4 tonnes in 2009.
In January 2010, hallmarks for palladium were introduced by assay offices in the United Kingdom, and it became a legal requirement to hallmark all articles of jewellery described as being wholly or partly made of palladium. Articles can be marked as containing a minimum of either 500, 950 or 999 parts per thousand of palladium. Fountain pen nibs made from gold are sometimes plated with palladium when a silver, rather than gold, appearance is desired. Sheaffer has used palladium plating for many decades, either as an accent on otherwise gold nibs or to cover the gold completely.
Finely divided palladium metal can be pyrophoric. As a platinum-group metal, the bulk material is quite inert. Although contact dermatitis has been reported, the amount of data on the effects of exposure to palladium is limited. It has been shown that people with an allergic reaction to palladium also react to nickel, making it advisable to avoid the use of dental alloys containing palladium on those so allergic.
A considerable amount of palladium is distributed by the exhausts of cars with catalytic converters. Between 4 and 108 ng/km of palladium particulate is released by such cars. Its total uptake from food is estimated to be lower than 2 µg per person a day. The second possible source for palladium is alloys for dental restoration, there the possible uptake of palladium is estimated to be lower than 15 µg per person per day. People working with palladium or its compounds might have a considerably higher uptake. For soluble compounds like palladium chloride 99% is eliminated from the body within 3 days.
- Magnetic susceptibility of the elements and inorganic compounds, in Lide, D. R., ed. (2005). CRC Handbook of Chemistry and Physics (86th ed.). Boca Raton (FL): CRC Press. ISBN 0-8493-0486-5.
- Hammond, C. R. (2004). The Elements, in Handbook of Chemistry and Physics 81st edition. CRC press. ISBN 0-8493-0485-7.
- Powers, D. C.; Ritter, T. (2011). "Palladium(III) in Synthesis and Catalysis". Top. Organomet. Chem. Topics in Organometallic Chemistry 35: 129–156. doi:10.1007/978-3-642-17429-2_6. ISBN 978-3-642-17428-5.
- Chen, W. (2002). "Synthesis and Structure of Formally Hexavalent Palladium Complexes". Science 295 (5553): 308. Bibcode:2002Sci...295..308C. doi:10.1126/science.1067027.
- Crabtree, R. H. (2002). "CHEMISTRY: A New Oxidation State for Pd?". Science 295 (5553): 288. doi:10.1126/science.1067921.
- "Atomic Weights and Isotopic Compositions for Palladium (NIST)". Retrieved 12 November 2009.
- Georges, Audi; Bersillon, O.; Blachot, J.; Wapstra, A.H. (2003). "The NUBASE Evaluation of Nuclear and Decay Properties". Nuclear Physics A (Atomic Mass Data Center) 729: 3–128. Bibcode:2003NuPhA.729....3A. doi:10.1016/j.nuclphysa.2003.11.001.
- Kelly, W. R.; Gounelle, G. J.; Hutchison, R. (1978). "Evidence for the existence of 107Pd in the early solar system". Geophysical Research Letters 359 (1787): 1079–1082. Bibcode:2001RSPTA.359.1991R. doi:10.1098/rsta.2001.0893.
- "Mexico's Meteorites". mexicogemstones.com.
- Chen, J. H.; Wasserburg, G. J. (1990). "The isotopic composition of Ag in meteorites and the presence of 107Pd in protoplanets". Geochimica et Cosmochimica Acta 54 (6): 1729–1743. Bibcode:1990GeCoA..54.1729C. doi:10.1016/0016-7037(90)90404-9.
- Craig, Bruce D.; Anderson, David S. (1995). "Atmospheric Environment". Handbook of corrosion data. ASM International. p. 126. ISBN 978-0-87170-518-1.
- Anderson, Gordon K.; Lin, Minren; Sen, Ayusman; Gretz, Efi (1990). "Bis(Benzonitrile)Dichloro Complexes of Palladium and Platinum". Inorganic Syntheses. Inorganic Syntheses 28: 60–63. doi:10.1002/9780470132593.ch13. ISBN 9780470132593.
- Zalevskaya, O. A.; Vorob’eva, E. G.; Dvornikova, I. A. and Kuchin, A. V. (2008). "Palladium complexes based on optically active terpene derivatives of ethylenediamine". Russian Journal of Coordination Chemistry 34 (11): 855–857. doi:10.1134/S1070328408110110.
- Mozingo, Ralph (1955), "Palladium Catalysts", Org. Synth.; Coll. Vol. 3: 685
- Miyaura, Norio and Suzuki, Akira (1993), "Palladium-catalyzed reaction of 1-alkenylboronates with vinylic halides: (1Z,3E)-1-Phenyl-1,3♫-octadiene", Org. Synth.; Coll. Vol. 8: 532
- Coulson, D. R.; Satek, L. C.; Grim, S. O. (1972). "23. Tetrakis(triphenylphosphine)palladium(0)". Inorg. Synth. Inorganic Syntheses 13: 121. doi:10.1002/9780470132449.ch23. ISBN 9780470132449.
- Takahashi, Y.; Ito, Ts.; Sakai, S.; Ishii, Y. (1970). "A novel palladium(0) complex; bis(dibenzylideneacetone)palladium(0)". Journal of the Chemical Society D: Chemical Communications (17): 1065. doi:10.1039/C29700001065.
- Crabtree, Robert H. (2009). "Application to Organic Synthesis". The Organometallic Chemistry of the Transition Metals. John Wiley and Sons. p. 392. ISBN 978-0-470-25762-3.
- Usselman, Melvyn (1978). "The Wollaston/Chenevix controversy over the elemental nature of palladium: A curious episode in the history of chemistry". Annals of Science 35 (6): 551–579. doi:10.1080/00033797800200431.
- Griffith, W. P. (2003). "Rhodium and Palladium – Events Surrounding Its Discovery". Platinum Metals Review 47 (4): 175–183.
- Wollaston, W. H. (1804). "On a New Metal, Found in Crude Platina". Philosophical Transactions of the Royal Society of London 94: 419–430. doi:10.1098/rstl.1804.0019.
- Wollaston, W. H. (1805). "On the Discovery of Palladium; With Observations on Other Substances Found with Platina". Philosophical Transactions of the Royal Society of London 95: 316–330. doi:10.1098/rstl.1805.0024.
- Garrett, Christine E.; Prasad, Kapa (2004). "The Art of Meeting Palladium Specifications in Active Pharmaceutical Ingredients Produced by Pd-Catalyzed Reactions". Advanced Synthesis & Catalysis 346 (8): 889–900. doi:10.1002/adsc.200404071.
- Williamson, Alan. "Russian PGM Stocks". The LBMA Precious Metals Conference 2003. The London Bullion Market Association. Retrieved 2 October 2010.
- "Historical Palladium Charts and Data". Kitco. Retrieved 2 October 2010.
- "Ford fears first loss in a decade". BBC News. 16 January 2002. Retrieved 19 September 2008.
- "Platinum-Group Metals". Mineral Commodity Summaries. United States Geological Survey. January 2007.
- Kielhorn, Janet; Melber, Christine; Keller, Detlef; Mangelsdorf, Inge (2002). "Palladium – A review of exposure and effects to human health". International Journal of Hygiene and Environmental Health 205 (6): 417–32. doi:10.1078/1438-4639-00180. PMID 12455264.
- "Why A Palladium Fund Has Launched In South Africa". Investing.com.
- "Platinum-Group Metals". Mineral Yearbook 2007. United States Geological Survey. January 2007.
- Verryn, Sabine M. C.; Merkle, Roland K. W. (1994). "Compositional variation of cooperite, braggite, and vysotskite from the Bushveld Complex". Mineralogical Magazine 58 (2): 223–234. doi:10.1180/minmag.1994.058.391.05.
- Genkin, A.D.; Evstigneeva, T.L. (1986). "Associations of platinum- group minerals of the Norilsk copper-nickel sulfide ores". Economic Geology 8l (5): 1203–1212. doi:10.2113/gsecongeo.81.5.1203.
- Kolarik, Zdenek; Renard, Edouard V. (2003). "Recovery of Value Fission Platinoids from Spent Nuclear Fuel. Part I PART I: General Considerations and Basic Chemistry". Platinum Metals Review 47 (2): 74–87.
- "Palladium". United Nations Conference on Trade and Development. Archived from the original on 6 December 2006. Retrieved 5 February 2007.
- Rushforth, Roy (2004). "Palladium in Restorative Dentistry: Superior Physical Properties make Palladium an Ideal Dental Metal". Platinum Metals Review 48 (1).
- Hesse, Rayner W. (2007). "palladium". Jewelry-making through history: an encyclopedia. Greenwood Publishing Group. p. 146. ISBN 978-0-313-33507-5.
- Toff, Nancy (1996). The flute book: a complete guide for students and performers. Oxford University Press. p. 20. ISBN 978-0-19-510502-5.
- Weithers, Timothy Martin (2006). "Precious Metals". Foreign exchange: a practical guide to the FX markets. p. 34. ISBN 978-0-471-73203-7.
- Tsuji, Jiro (2004). Palladium reagents and catalysts: new perspectives for the 21st century. John Wiley and Sons. p. 90. ISBN 0-470-85032-9.
- Drahl, Carmen (2008). "Palladium's Hidden Talent". Chemical & Engineering News 86 (35): 53–56. doi:10.1021/cen-v086n035.p053.
- Brown, William Henry; Foote, Christopher S; Iverson, Brent L (2009). "Catalytic reduction". Organic chemistry. Cengage Learning. p. 270. ISBN 978-0-495-38857-9.
- Zogbi, Dennis (3 February 2003). "Shifting Supply and Demand for Palladium in MLCCs". TTI, Inc.
- Mroczkowski, Robert S. (1998). Electronic connector handbook: theory and applications. McGraw-Hill Professional. pp. 3–. ISBN 978-0-07-041401-3.
- Harper, Charles A. (1997). Passive electronic component handbook. McGraw-Hill Professional. pp. 580–. ISBN 978-0-07-026698-8.
- Jollie, David (2007). "Platinum 2007" (PDF). Johnson Matthey.
- Morton, Linda Palladium sorbents remove contaminants from syngas, DOE Pulse, Number 335, 18 April 2011
- Shu, J.; Grandjean, B. P. A.; Neste, A. Van; Kaliaguine, S. (1991). "Catalytic palladium-based membrane reactors: A review". The Canadian Journal of Chemical Engineering 69 (5): 1036. doi:10.1002/cjce.5450690503.
- Allen, TH; Root, WS (1955). "An improved palladium chloride method for the determination of carbon monoxide in blood". The Journal of Biological Chemistry 216 (1): 319–323. PMID 13252031.
- Manchester, F. D.; San-Martin, A.; Pitre, J. M. (1994). "The H-Pd (hydrogen-palladium) System". Journal of Phase Equilibria 15: 62. doi:10.1007/BF02667685.
- Greenwood, Norman N.; Earnshaw, Alan (1997). Chemistry of the Elements (2nd ed.). Butterworth-Heinemann. pp. 1150–151. ISBN 0080379419.
- Grochala, W.; Edwards, P. P. (2004). "Thermal Decomposition of the Non-Interstitial Hydrides for the Storage and Production of Hydrogen". Chemical Reviews 104 (3): 1283–1316. doi:10.1021/cr030691s. PMID 15008624.
- Gupta, Dinesh C.; Langer, Paul H.; ASTM Committee F-1 on Electronics (1987). Emerging semiconductor technology: a symposium. ASTM International. pp. 273–. ISBN 978-0-8031-0459-4.
- Miller, William Allen (1868). Elements of chemistry: theoretical and practical. Wiley. pp. 711–.
- Hindsén, M.; Spirén, A.; Bruze, M. (2005). "Cross-reactivity between nickel and palladium demonstrated by systemic administration of nickel". Contact Dermatitis 53 (1): 2–8. doi:10.1111/j.0105-1873.2005.00577.x. PMID 15982224.
- "Daily Metal Prices: September 2001". Johnson Matthey.
- Holmes, E. (13 February 2007). "Palladium, Platinum's Cheaper Sister, Makes a Bid for Love". Wall Street Journal (Eastern edition). pp. B.1.
- "Platinum-Group Metals". Mineral Yearbook 2009. United States Geological Survey. January 2007.
- "Platinum-Group Metals". Mineral Yearbook 2006. United States Geological Survey. January 2007.
- Ware, Mike (2005). "Book Review of : Photography in Platinum and Palladium". Platinum Metals Review 49 (4): 190–195. doi:10.1595/147106705X70291.
- Zereini, Fathi; Alt, Friedrich (2006). "Health Risk Potential of Palladium". Palladium emissions in the environment: analytical methods, environmental assessment and health effects. Springer Science & Business. pp. 549–563. ISBN 978-3-540-29219-7.
- Wataha, J.C.; Hanks, C.T. (1996). "Biological effects of palladium and risk of using palladium in dental casting alloys". Journal of Oral Rehabilitation 23 (5): 309–20. doi:10.1111/j.1365-2842.1996.tb00858.x. PMID 8736443.
- Aberer, Werner; Holub, Henriette; Strohal, Robert; Slavicek, Rudolf (1993). "Palladium in dental alloys – the dermatologists' responsibility to warn?". Contact Dermatitis 28 (3): 163–5. doi:10.1111/j.1600-0536.1993.tb03379.x. PMID 8462294.
- Wataha, John C; Shor, Kavita (2010). "Palladium alloys for biomedical devices". Expert Review of Medical Devices 7 (4): 489–501. doi:10.1586/erd.10.25. PMID 20583886.
|Wikimedia Commons has media related to Palladium.|
|Look up palladium in Wiktionary, the free dictionary.|
- Palladium at The Periodic Table of Videos (University of Nottingham)
- Current and Historical Palladium Price
- Special Market Report on Palladium and Precious Metals
|Periodic table (Large version)|